**HAL Id: hal-02738157**

**https://hal.archives-ouvertes.fr/hal-02738157**

### Submitted on 2 Jun 2021

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

### Distributed under a Creative Commons Attribution| 4.0 International License

**Computer-Generated Glasses**

### Dmytro Khomenko, Camille Scalliet, Ludovic Berthier, David Reichman,

### Francesco Zamponi

**To cite this version:**

### Dmytro Khomenko, Camille Scalliet, Ludovic Berthier, David Reichman, Francesco Zamponi.

### De-pletion of Two-Level Systems in Ultrastable Computer-Generated Glasses. Physical Review Letters,

### American Physical Society, 2020, 124 (22), �10.1103/PhysRevLett.124.225901�. �hal-02738157�

### Depletion of two-level systems in ultrastable computer-generated glasses

Dmytro Khomenko*,1, 2 _{Camille Scalliet*,}3,∗ _{Ludovic Berthier,}4, 5 _{David R. Reichman,}2 _{and Francesco Zamponi}1

1_{Laboratoire de Physique de l’Ecole Normale Sup´erieure, ENS, Universit´e PSL,}
CNRS, Sorbonne Universit´e, Universit´e de Paris, 75005 Paris, France
2_{Department of Chemistry, Columbia University, New York, NY 10027, USA}

3_{DAMTP, Centre for Mathematical Sciences, University of Cambridge,}
Wilberforce Road, Cambridge CB3 0WA, United Kingdom

4_{Department of Chemistry, University of Cambridge,}
Lensfield Road, Cambridge CB2 1EW, United Kingdom

5_{Laboratoire Charles Coulomb (L2C), Universit´e de Montpellier, CNRS, 34095 Montpellier, France}
(Dated: June 17, 2020)

Amorphous solids exhibit quasi-universal low-temperature anomalies whose origin has been
as-cribed to localized tunneling defects. Using an advanced Monte Carlo procedure, we create in silico
glasses spanning from hyperquenched to ultrastable glasses. Using a multidimensional path-finding
protocol, we locate tunneling defects with energy splittings smaller than kBTQ, with TQ the
tem-perature below which quantum effects are relevant (TQ_{≈ 1 K in most experiments). We find that}
as the stability of a glass increases, its energy landscape as well as the manner in which it is probed
tend to deplete the density of tunneling defects, as observed in recent experiments. We explore the
real-space nature of tunneling defects, and find that they are mostly localized to a few atoms, but
are occasionally dramatically delocalized.

The theory of low-temperature properties of perfect
crystals stands as one of the most profound early tests
of the power of quantum statistical mechanics. In
par-ticular, Debye’s calculation of the observed T3 _{}

behav-ior of the low-temperature specific heat highlighted the
importance of long wavelength phonons as low energy
excitations in ordered solids [1]. Given that the
wave-length of populated phonon modes around T _{∼ 1 K is}
significantly longer than the interparticle distance in a
solid, it came as a major surprise in 1971 when Zeller and
Pohl [2] measured large deviations from the expected
De-bye behavior of the specific heat and the thermal
conduc-tivity of vitreous silica, selenium and germanium-based
glasses. An explanation for this puzzling observation was
almost immediately put forward by Anderson, Halperin
and Varma [3], and Phillips [4]. They posited that the
disorder intrinsic to amorphous solids causes their energy
landscape to have many minima. Rare, nearly
degener-ate, adjacent local minima support tunneling defects or
two-level systems (TLS) with energy splittings of the
or-der of 1 K, which provide a large excess contribution to
the specific heat and a new mode of scattering that
de-termines the thermal conductivity. In the subsequent
decades, the behavior described by Zeller and Pohl was
observed in numerous other amorphous materials, and
the TLS theory has withstood essentially all experimental
tests [5–9]. Despite this great progress, the microscopic
real-space structure of the tunneling defects remains
de-bated, as do the factors that determine their density and
distribution in amorphous solids [10–22].

*Equal contribution to the work

A powerful platform for addressing these issues is the use of computer simulation to prepare amorphous materi-als in silico and to interrogate the simulated energy land-scape for TLS [23]. This program was initiated by Still-inger and Weber [24, 25], then carried out more exten-sively by Heuer and Silbey [26–29], nearly three decades ago. Limited by the computational power and algorithms available back then, they created computer glasses with cooling rates roughly nine orders of magnitude larger than in laboratory settings. They were able to locate only a handful of TLS with the requisite tunnel splittings, necessitating uncontrolled extrapolations. The situation then improved incrementally [30–33], although the algo-rithmic ability to simulate glasses which are cooled in an experimentally realistic way has remained out of reach until very recently. This limited greatly our microscopic understanding of the universal anomalous thermal be-havior of low-temperature glasses from a computational viewpoint.

In this work we leverage the remarkable ability of the swap Monte Carlo algorithm to produce in silico amor-phous materials with fictive temperatures that range from those found in typical experiments to the signifi-cantly slower rates found in recent vapor deposition stud-ies [34]. We find a dramatic depletion of active TLS (those with a tunnel splitting ∼ 1 K) with decreasing quench rate, as found in recent experiments [35–39], with the notable exception of old amber glasses [40]. We use a state-of-the-art reaction path-finding protocol [41, 42] to efficiently locate double-well potentials in the multi-dimensional potential energy landscape, yielding a direct sampling of tunneling states with sufficient statistics to avoid any extrapolation. We determine the degree of

FIG. 1. (a) Glasses are prepared at equilibrium (black line)
at temperatures Tf = 0.092, 0.07, 0.062 (bullets), from
hyper-quenched to ultrastable. We follow their potential energy
af-ter rapid quenches (colored lines). (b) Sketch of the potential
energy landscape. Double-well potentials are detected with
molecular dynamics simulations at TMD= 0.04 (blue). (c) A
detected double-well potential V (ξ). The classical asymmetry
∆V , activation energy Va, energy barrier Vb = Va_{− ∆V/2,}
the energy levels,E1andE2, of the ground-state doublet, and
the tunnel splitting, E =_{E}2− E1, are illustrated.

localization of individual TLS, providing a detailed, real-space understanding of how atoms participate in tun-neling motion and how the thermal exploration of the energy landscape in well-annealed amorphous materials determines the density of tunneling centers.

Glass preparation – Past works on the landscape of low-temperature glasses focused on simple models for real materials such as NiP [26], Argon [30], and silica [32,33]. Our goal is to understand how glass preparation affects the density of TLS, within a single model. We study a polydisperse mixture of particles interacting via an in-verse power law potential [34]. Our choice is motivated by the fact that low-temperature anomalies are observed in glasses, regardless the material. Given the diversity of models, we choose one for which swap Monte Carlo enables maximally efficient thermalization on the com-puter over a range of temperatures at least as wide as in experiments [34].

We provide minimal details on the system and mea-sures of equilibration (see SI for details). We simulate a non-additive polydisperse mixture of N = 1500 particles of mass m. Two particles i and j separated by a distance rij interact via the potential

v(rij) = σij rij 12 + F (rij/σij) (1)

only if rij < rcut = 1.25σij, σij being the non-additive

interaction length scale. The function F is a fourth-order polynomial which guarantees continuity of the po-tential up to the second derivative at rcut. We

charac-terize the physical classical dynamics of the model
us-ing molecular dynamics (MD) with energies and lengths
expressed in units of and the average diameter σ,
re-spectively. Times measured during MD simulations are
expressed in units ofp/mσ2_{. Number density is set to}

ρ = 1. The relaxation time τα of the equilibrium fluid is

measured from the self-intermediate scattering function Fs(k = 7.0, τα) = e−1. The onset of glassy dynamics,

sig-naled by deviations from Arrhenius behavior, takes place at To= 0.18, where τα(To)≡ τo, and the mode-coupling

crossover temperature is TM CT = 0.104 [34].

We analyze in silico glasses by preparing fully equi-librated configurations at various preparation tempera-tures Tf using the swap Monte Carlo algorithm, which

utilizes the exchange of particles’ diameters in addition to standard translational moves, leading to a massive thermalization speed-up. Our implementation is that of Ref. [43]. The configurations are then rapidly cooled to lower temperatures using regular molecular dynamics. Therefore, Tf represents the “temperature at which the

glass would find itself in equilibrium if suddenly brought to it from its given state,” which is precisely the defini-tion of Tool’s fictive temperature [44]. The temperature Tf characterizes the degree of stability of the glasses,

see Fig.1(a). In experiments, Tf would be determined

by the cooling rate [45, 46], or the substrate temper-ature in a vapor deposition experiment [47–51]. We present results for glasses in wide range of stabilities: poorly annealed (hyperquenched) glasses (Tf = 0.092

where log(τα/τo) = 4.9, slightly below TM CT),

liquid-cooled experimental glasses (Tf = 0.07 ' Tg, where

log(τα/τo) = 10.7), and ultrastable glasses (Tf = 0.062,

where log(τα/τo) = 14.8). To obtain statistically

signifi-cant results, we analyze Ng independent samples (Ng =

200, 50, 15 for increasing Tf).

Landscape exploration – We identify transitions be-tween nearby minima, or double well potentials (DWPs) in the glasses. Briefly, starting from the configurations equilibrated at Tf, we run MD simulations at TMD =

0.04, which is sufficiently low to confine each glass in a single metabasin, but high enough that the system can rapidly visit distinct minima (inherent structures) within the metabasin [23], see Fig.1(b). Details are given in the SI.

3

FIG. 2. Probability distribution functions of DWP param-eters as a function of glass preparation temperature Tf: (a) asymmetry ∆V , (b) energy barrier Vb, (c) distance d nor-malized by√P R, which characterizes the typical individual displacement of particles that participate actively in a double-well transition, and (d) participation ratio P R. Lines are a guide for the eye.

By sampling the inherent structures along MD trajec-tories [30], we obtain a library of visited minima, as well as the pairs of them that are dynamically connected. We use the isoconfigurational ensemble [52]: for each of the Ng independent configurations, we run up to 200 MD

simulations, each initialized with different velocities. The number and duration of isoconfigurational runs is large enough for the probability distribution function (pdf) of the inherent structures potential energy, and the number of transitions, to reach stationarity. While we reach con-vergence of the pdfs, all possible minima are not sampled, and their numbers increase with additional runs. We however sample a significant number of minima: 13252, 26898, 848698 for Tf = 0.062, 0.07, 0.092, respectively.

As shown below, this is enough to directly determine the density of tunneling TLS.

We select transitions between adjacent minima as de-scribed in the SI. We compute the minimum energy path connecting each pair of minima using a climbing image Nudged Elastic Band (NEB) algorithm [41, 42], which ensures the accurate determination of the saddle point, and provides a smooth energy profile. Occasionally, espe-cially for Tf = 0.092, the NEB energy profile contains

in-termediate minima. In such cases, we apply an iterative method to split the energy profile into distinct DWPs, which are then analyzed similarly to the other ones.

We parametrize a DWP by its potential energy V (ξ)
along the minimum energy path, with ξ = 0, 1
corre-sponding to the two minima (we arbitrarily choose ξ = 0
for the deepest minimum), see Fig.1(c). A DWP is
char-acterized by its asymmetry ∆V = V (1)_{− V (0), energy}
barrier Vb= Va−∆V/2, where Vais the activation energy,

FIG. 3. Cumulative distribution of energy splitting n(E) di-vided by E, from hyperquenched to ultrastable glasses (top to bottom). The values m are chosen for comparison withe real materials. The plateau at small E affords a direct deter-mination of the TLS density n0, which is suppressed by two orders of magnitude as glass preparation is varied.

and the distance d between minima. The distance is
cal-culated along the reaction coordinate given by the NEB,
as the sum of Euclidean distances between images of the
system: d2 _{=} P

i,µd2i,µ, where di,µ is the displacement

of particle i in direction µ = x, y, z. The participation
ratio, P R = d4_{/(}P

i,µd4i,µ), characterizes the number of

particles involved in the transition.

We present in Fig.2the statistics of the DWP param-eters. The pdfs for Tf = 0.062 and 0.07 agree

quanti-tatively, within noise, while we observe an evolution for Tf = 0.092. In particular, the pdfs of asymmetries and

energy barriers are almost exponential in all glasses. The mild dependence of these tails on Tf may stem from the

fact that the sampling temperature TMD sets a limit on

the DWPs that can be detected, independently of Tf(see

SI for the effect of TMD). While the distribution of

en-ergy asymmetry is exponential at high energies ∆V , it becomes flat at low energies where TLS are found (see Fig. S6). The pdfs of distances (not shown) and partic-ipation ratios vary more significantly between Tf ≤ 0.07

and Tf = 0.092. Since d∝

√

P R, an increase of P R will affect the distribution of d. We instead study the pdf of d/√P R. This quantity can be interpreted as an aver-age displacement of the particles that participate in the transition. On average, the number of particles involved in DWPs is larger in poorly annealed glasses, while the displacements of individual particles remain comparable. To our knowledge, the dependence of the quench rate on DWPs classical parameters has not yet been reported. Note that TLS typically correspond to DWPs with very small ∆V and relatively large Vb. The tunnel splitting

stems from non-trivial correlations between the classi-cal parameters [30], thus the pdfs of classical parameters alone are not informative on quantum tunneling (see SI). Density of two-level systems – At sufficiently low tem-peratures, thermal activation over the energy barrier Vb

is suppressed, and quantum tunneling becomes
impor-tant [53]. In our analysis, we reduce the problem to a one
dimensional effective Schr¨odinger equation along the
re-action coordinate. Following Vineyard [54], the effective
mass remains m, with a reaction coordinate x _{∈ [0, d].}
Using the normalized variable ξ = x/d, and scaling
ener-gies by , we obtain
− ~
2
2md2_{}∂
2
ξΨ(ξ) + V (ξ)Ψ(ξ) =EΨ(ξ), (2)

where the “quantumness” of the problem is controlled
by the dimensionless mass m = mσ_{e} 2_{/}_{~}2 _{(see Fig.} _{3}_{).}

In general, the Laplacian should take into account cur-vature effects, which we neglect here.The potential V (ξ) obtained from the NEB is defined in ξ∈ [0, 1]. To solve Eq. (2), we extrapolate it outside this interval (see SI).

We solve Eq. (2) for all DWPs. We compute the first two energy levels,E1 and E2, of the double well and

de-fine the tunnel splitting E = E2 − E1. We illustrate

in Fig. 1(c) the two energy levels and tunnel splitting
of a DWP. The tunnel splitting E is the relevant
pa-rameter for low-temperature properties. The transitions
that occur by quantum tunneling have a tunnel splitting
E _{∼ T [}6]. These particular DWPs are called tunneling
two-level systems (TLS).

We characterize the distribution of TLS using a cumu-lative distribution of tunnel splittings n(E), defined as the number of DWPs with tunnel splitting smaller than E, normalized by the number of particles N in the glass, and the number of independent samples Ng. In TLS

the-ory, n(E) can be expanded as n(E)' n0E +O(E2) for

small E, the specific heat at low temperature is linear with T , and n0 enters the prefactor [3,6].

In order to estimate the density n0 of TLS and its

de-pendence on glass stability, we plot n(E)/E as a function of tunnel splitting E in Fig.3. All curves indicate a sat-uration to a plateau value, n0, at low E. The existence

of a plateau value demonstrates our ability to directly estimate the density of TLS n0without any uncontrolled

extrapolation. Data on tunneling rates [55] and distri-bution of tunneling matrix elements ∆0 are presented in

the SI.

Our key result is that the TLS density n0(as estimated

by n(E)/E in the range 10−3_{− 10}−4_{) decreases by two}

orders of magnitude from hyperquenched to ultrastable glasses. To our knowledge, this constitutes the first nu-merical evidence for a significant suppression of TLS with increasing glass stability.

Microscopic nature of TLS – How many particles are
involved in the tunneling motion of a TLS? [30–33] We
analyzed how the participation ratio of transitions
cor-relates with the tunnel splitting E. We find that the
participation ratio of low-temperature active TLS with
tunnel splittings E _{∼ 10}−3_{− 10}−4 _{varies from 1 to 200}

(see SI). The higher participation ratios (P R _{∼ 200)}
are found in hyperquenched glasses, while in ultrastable

(a) (b)

FIG. 4. Snapshots of TLS with low tunnel splitting E for Tf =
0.092 andm = 30000. (a) P R_{e} _{≈ 126 with E = 8.9×10}−5_{. (b)}
P R_{≈ 1.6 and similarly low E = 5.4×10}−5. The size and color
of particles are proportional to their displacement between the
initial and final configurations of the TLS, normalized to the
highest displacement.

glasses the participation ratio rarely exceeds _{∼ 30. We}
provide systematic numerical evidence that TLS active
at low temperature are typically very localized, but
oc-casionally associated with collective excitations. We
pro-vide two snapshots in Fig.4, corresponding to a collective
TLS (left) and a very localized TLS (right) identified in
a hyperquenched glass.

Discussion – Our study of tunneling TLS in a sim-ple computer model demonstrates their importance to understand low-temperature glass anomalies. We show that the density n0 of TLS directly controls the linear

temperature dependence of the specific heat at low tem-peratures. Several recent works advocated the idea that quantized low-frequency harmonic modes alone could ex-plain this behavior [10,18,56–60]. These soft modes are known for our glasses [61], but we find that their contri-bution to the low-temperature specific heat is subdomi-nant (see SI), suggesting that the specific heat of struc-tural glasses is dominated by tunneling TLS, as originally proposed in [3,6].

To relate our data to experiments we convert simula-tion units into physical ones. The temperature scale be-low which quantum effects become important is obtained by comparing the thermal wavelength to the interparti-cle distance: TQ = 2π~

2

mσ2_{k}

B. We consider DWPs with

E < kBTQ as low-temperature active TLS, and their

to-tal number is nactive= N Ngn(E = kBTQ).

A detailed analysis on experimental comparisons is
presented in the SI. We first consider Argon
parame-ters: σ = 3.4× 10−10_{m, /4 = 1.65}_{× 10}−21_{J, m =}

6× 10−26_{kg [}_{30}_{]. This gives T}

g ∼ 32 K, TQ ∼ 0.73 K,

andme ∼ 4000. For this choice, we estimate from Fig.3

nsim0 ∼ 4, 0.4, 0.04 for increasing glass stability. This

gives nexp_{0} _{∼ 10}49_{, 10}48_{, 10}47 _{J}−1_{m}−3_{. Active TLS have}

E < kBTQ = 0.0015 and we find nactive = 1008, 291,

5 A second choice motivated by NiP metallic glasses [26]

would be to use Nickel as a reference, for which σ =
2.21_{×10}−10_{m, = 6.14}_{×10}−20_{J, m = 1.02}_{×10}−25_{kg [}_{62}_{].}

In this case, we have Tg ∼ 298 K, TQ ∼ 0.9 K, and em∼

30000. For this value ofm, we find n_{e} sim

0 ∼ 60, 6, 0.6 for

Tf = 0.092, 0.07, 0.062, yielding nexp0 ∼ 1050, 1049, 1048

J−1_{m}−3_{. Active TLS have E < k}

BTQ = 0.0002 and we

find nactive= 248, 46, 28 such TLS for Tg= 0.092, 0.07,

0.062, respectively.

Experimentally, a value of n0 ∼ 1046J−1m−3 is

re-ported [6, 7]. Our estimation for Tf = 0.07 is larger

by a factor_{∼ 10}2

− 103 _{(Argon and Nickel, respectively).}

It is difficult to rationalize this discrepancy but we can offer several hypothesis. One possibility is that we in-clude in our estimates all DWPs detected at temperature TMD= 0.04 TQ, while experimentally, the glass is

di-rectly brought to TQ and only a small fraction of TLS

that lie at the bottom of the energy metabasin would be excited. Furthermore, not all TLS would tunnel on the relevant timescales: it is known that n0 ∼ log(τ) where

τ is the observation time at TQ [6]. This should persist

up to the timescale of complete exploration of the en-ergy landscape. Our exploration protocol at TMD TQ

artificially sets τ larger than this cutoff (see SI for the tunneling rates of TLS). Another explanation could be that our model is too simple to describe real molecular materials, for example network glasses. Since we analyze a single model, the fundamental question of universality in TLS density remains unanswered. Analyzing differ-ent glass-forming models will be crucial to answer this question.

The reduction of n0 by two orders of magnitude

when moving from hyperquenched to ultrastable glasses is robust and in good agreement with recent experi-ments [36, 39]. We show that for a given glass-forming model, glass preparation affects dramatically the density of TLS. Our results demonstrate that glass ultrastability (rather than potential anisotropy of the vapor-deposited samples) is responsible for the depletion of TLS.

We thank M. Ediger, D. Rodney and W. Ji for discus-sions. This project received funding from the European Research Council (ERC) under the European Union’s Horizon 2020 research and innovation program, Grant No. 723955 – GlassUniversality (FZ), and Grant No. 740269 –ADNeSP (Prof. M. E. Cates), and from the Si-mons Foundation (#454933, LB, #454955, FZ, #454951 DR). CS acknowledges the Fondation l’Or´eal.

∗ _{cs2057@cam.ac.uk}

[1] N. W. Ashcroft and N. D. Mermin, Solid State Physics (Thomson Learning, 1976).

[2] R. C. Zeller and R. O. Pohl,Phys. Rev. B 4, 2029 (1971).

[3] P. W. Anderson, B. I. Halperin, and C. M. Varma, Philo-sophical Magazine 25, 1 (1972).

[4] W. Phillips,Journal of Low Temperature Physics 7, 351 (1972).

[5] M. T. Loponen, R. C. Dynes, V. Narayanamurti, and J. P. Garno,Physical Review B 25, 1161 (1982). [6] W. A. Phillips, Reports on Progress in Physics 50, 1657

(1987).

[7] J. F. Berret and M. Meißner, Zeitschrift f¨ur Physik B Condensed Matter 70, 65 (1988).

[8] A.-M. Boiron, P. Tamarat, B. Lounis, R. Brown, and M. Orrit,Chemical physics 247, 119 (1999).

[9] A. L. Burin, J. M. Leveritt III, G. Ruyters, C. Sch¨otz, M. Bazrafshan, P. Fassl, M. von Schickfus, A. Fleis-chmann, and C. Enss,EPL (Europhysics Letters) 104, 57006 (2013).

[10] Y. M. Galperin, V. Karpov, and V. Kozub, Advances in Physics 38, 669 (1989).

[11] S. N. Coppersmith,Phys. Rev. Lett. 67, 2315 (1991). [12] A. J. Leggett,Physica B: Condensed Matter 169, 322

(1991).

[13] A. Burin and Y. Kagan, Physics Letters A 215, 191 (1996).

[14] D. R. Reichman, P. Neu, and R. J. Silbey, Molecular Crystals and Liquid Crystals Science and Technology. Section A. Molecular Crystals and Liquid Crystals 291, 65 (1996).

[15] V. Lubchenko and P. G. Wolynes,Phys. Rev. Lett. 87, 195901 (2001).

[16] V. Gurarie and J. T. Chalker,Phys. Rev. B 68, 134207 (2003).

[17] V. Lubchenko and P. G. Wolynes, Proceedings of the National Academy of Sciences 100, 1515 (2003). [18] D. A. Parshin, H. R. Schober, and V. L. Gurevich,Phys.

Rev. B 76, 064206 (2007).

[19] D. C. Vural and A. J. Leggett,Journal of Non-Crystalline Solids 357, 3528 (2011).

[20] A. J. Leggett and D. C. Vural,The Journal of Physical Chemistry B 117, 12966 (2013), pMID: 23924397. [21] D. Zhou and A. J. Leggett,arXiv:1510.05538 (2015). [22] H. M. Carruzzo and C. C. Yu, Phys. Rev. Lett. 124,

075902 (2020).

[23] A. Heuer, Journal of Physics: Condensed Matter 20, 373101 (2008).

[24] F. H. Stillinger and T. A. Weber,Physical Review A 25, 978 (1982).

[25] T. A. Weber and F. H. Stillinger,Physical Review B 32, 5402 (1985).

[26] A. Heuer and R. J. Silbey, Phys. Rev. Lett. 70, 3911 (1993).

[27] A. Heuer and R. J. Silbey,Phys. Rev. B 49, 1441 (1994). [28] D. Dab, A. Heuer, and R. Silbey,Journal of

Lumines-cence 64, 95 (1995).

[29] A. Heuer and R. J. Silbey,Phys. Rev. B 53, 609 (1996). [30] F. Demichelis, G. Viliani, and G. Ruocco,

PhysChem-Comm 2, 20 (1999).

[31] J. Reinisch and A. Heuer, Phys. Rev. B 70, 064201 (2004).

[32] J. Reinisch and A. Heuer,Phys. Rev. Lett. 95, 155502 (2005).

[33] T. Damart and D. Rodney, Phys. Rev. B 97, 014201 (2018).

[34] A. Ninarello, L. Berthier, and D. Coslovich, Physical Review X 7, 021039 (2017).

[35] D. R. Queen, X. Liu, J. Karel, T. H. Metcalf, and F. Hell-man,Phys. Rev. Lett. 110, 135901 (2013).

[36] T. P´erez-Casta˜neda, C. Tinoco, J. Rodr´ıguez-Viejo, and M. A. Ramos, Proceedings of the National Academy of Sciences 111, 11275 (2014).

[37] X. Liu, D. R. Queen, T. H. Metcalf, J. E. Karel, and F. Hellman,Phys. Rev. Lett. 113, 025503 (2014). [38] M. D. Ediger,Proceedings of the National Academy of

Sciences 111, 11232 (2014).

[39] D. R. Queen, X. Liu, J. Karel, H. C. Jacks, T. H. Metcalf, and F. Hellman,Journal of Non-Crystalline Solids 426, 19 (2015).

[40] T. P´erez-Casta˜neda, R. J. Jim´enez-Riob´oo, and M. A. Ramos,Phys. Rev. Lett. 112, 165901 (2014).

[41] H. J´onsson, G. Mills, and K. W. Jacobsen, in Classi-cal and Quantum Dynamics in Condensed Phase Simu-lations, edited by B. J. Berne, G. Ciccotti, and D. F. Coker (World Scientific, Singapore, 1998).

[42] G. Henkelman, B. P. Uberuaga, and H. J´onsson, The Journal of chemical physics 113, 9901 (2000).

[43] L. Berthier, E. Flenner, C. J. Fullerton, C. Scalliet, and M. Singh,Journal of Statistical Mechanics: Theory and Experiment 2019, 064004 (2019).

[44] A. Q. Tool,Journal of the American Ceramic society 29, 240 (1946).

[45] M. D. Ediger, C. A. Angell, and S. R. Nagel,The Journal of Physical Chemistry 100, 13200 (1996).

[46] A. Cavagna,Physics Reports 476, 51 (2009).

[47] S. F. Swallen, K. L. Kearns, M. K. Mapes, Y. S. Kim, R. J. McMahon, M. D. Ediger, T. Wu, L. Yu, and S. Satija,Science 315, 353 (2007).

[48] K. L. Kearns, S. F. Swallen, M. D. Ediger, T. Wu, Y. Sun, and L. Yu, The Journal of Physical Chemistry B 112, 4934 (2008).

[49] M. Tylinski, Y. Chua, M. Beasley, C. Schick, and M. Edi-ger,The Journal of chemical physics 145, 174506 (2016). [50] M. D. Ediger, The Journal of Chemical Physics 147,

210901 (2017).

[51] J. R`afols-Rib´e, M. Gonzalez-Silveira, C. Rodr´ıguez-Tinoco, and J. Rodr´ıguez-Viejo, Physical Chemistry Chemical Physics 19, 11089 (2017).

[52] A. Widmer-Cooper, P. Harrowell, and H. Fynewever,

Phys. Rev. Lett. 93, 135701 (2004).

[53] M. J. Gillan,Journal of Physics C: Solid State Physics 20, 3621 (1987).

[54] G. H. Vineyard, Journal of Physics and Chemistry of Solids 3, 121 (1957).

[55] A. Andreassen, D. Farhi, W. Frost, and M. D. Schwartz,

Phys. Rev. D 95, 085011 (2017).

[56] L. Gil, M. A. Ramos, A. Bringer, and U. Buchenau,

Phys. Rev. Lett. 70, 182 (1993).

[57] D. A. Parshin,Phys. Rev. B 49, 9400 (1994).

[58] W. Ji, M. Popovi´c, T. W. J. de Geus, E. Lerner, and M. Wyart,Phys. Rev. E 99, 023003 (2019).

[59] S. Franz, T. Maimbourg, G. Parisi, and A. Scardicchio,

Proceedings of the National Academy of Sciences 116, 13768 (2019).

[60] M. Baggioli, R. Milkus, and A. Zaccone,

arXiv:1903.05237 (2019).

[61] L. Wang, A. Ninarello, P. Guan, L. Berthier, G. Szamel, and E. Flenner,Nature communications 10, 26 (2019). [62] W. Ching and C. C. Lin, in Amorphous Magnetism II

### Supplemental Material: Depletion of two-level systems in ultrastable

### computer-generated glasses

Dmytro Khomenko*,1 _{Camille Scalliet*,}2 _{Ludovic Berthier,}3, 4 _{David R. Reichman,}5 _{and Francesco Zamponi}1

1_{Laboratoire de Physique de l’Ecole Normale Supérieure, ENS, Université PSL,}
CNRS, Sorbonne Université, Université de Paris, 75005 Paris, France

2_{Department of Applied Mathematics and Theoretical Physics,}

University of Cambridge, Wilberforce Road, Cambridge CB3 0WA, United Kingdom
3_{Department of Chemistry, University of Cambridge,}

Lensfield Road, Cambridge CB2 1EW, United Kingdom

4_{Laboratoire Charles Coulomb (L2C), Université de Montpellier, CNRS, 34095 Montpellier, France}
5_{Department of Chemistry, Columbia University, New York, NY 10027, USA}

(Dated: June 17, 2020)

I. MODEL

We study a three-dimensional, non-additive, continuously polydisperse mixture of particles interacting via the pair potential Eq. (1) (main text). The particle diameters σi are drawn from the normalized distribution P (0.73 < σ <

1.62) ∼ 1/σ3_{, with average diameter hσi =} R _{P (σ)dσ = 1} _{(simply denoted as σ in the main text). We employ a}

non-additive cross-diameter σij = 0.5(σi+ σj) (1− 0.2|σi− σj|). This model is efficiently simulated with the swap

Monte Carlo algorithm. The choice of particle dispersity and non-additivity make the homogeneous fluid robust against fractionation and crystallization at all temperatures numerically explorable [S1]. As in the main text, classical quantities are given in units of , σ, m.

We characterize the dynamic slowdown of the supercooled liquid using molecular dynamics (MD) simulations. The temperature evolution of the relaxation time ταprovides three temperatures relevant to this work. The onset of glassy

dynamics, signaled by deviations from Arrhenius behavior, takes place at To= 0.18, where τα(To) = τo. The

mode-coupling crossover temperature TM CT = 0.104is measured by fitting the relaxation time data to τα∼ (T − TM CT)−γ

in a limited window of relatively high temperatures. At TM CT, the dynamics is four orders of magnitude slower than

at the onset temperature, τα(TM CT) ' 104τo. We take TM CT as a proxy for the computer glass transition, below

which standard MD fail to equilibrate the homogeneous fluid. The experimental glass transition Tg= 0.067is located

by fitting the relaxation time data to a parabolic law, using τα(Tg) = 1012τo [S1].

This glass-forming model is efficiently simulated at equilibrium with the swap Monte Carlo algorithm. We employ the swap Monte Carlo algorithm implemented in the LAMMPS package, with the optimal parameters, as described in Ref. [S2]. Supercooled liquid configurations can be generated down to T = 0.062, i.e. below the experimental glass transition Tg. In this work, we focus on configurations prepared in equilibrium conditions at temperatures Tf =

0.092, 0.07, 0.062. For the two lowest Tf values, standard MD dynamics initialized from an equilibrium configuration

is completely arrested: no diffusion is observed and the system is trapped within a glass metabasin. For the higher Tf= 0.092, some diffusion is observed in equilibrium; but if the system is rapidly cooled at lower temperatures, once

again no diffusion is observed and a glass state is obtained. Borrowing from experimental conventions [S3], we call this the “fictive temperature” of the glasses, as discussed in the main text.

II. LANDSCAPE EXPLORATION

The amorphous configurations generated at Tf are first thermalized to TMD= 0.04 using a Berendsen thermostat.

At this temperature, no diffusion is observed for all glasses. The system is then simulated in the NVE ensemble, using an integration time step of dt = 0.01. Configurations along the MD trajectory are used as the starting point for energy minimization via a conjugate gradient algorithm, which brings them to their inherent structure (IS), i.e. the nearest local minimum in the potential energy landscape (PEL). Note that contrary to the MD simulations, the minimization procedure does not conserve the total energy. We minimize the MD configurations obtained every 20, 10, 5 time steps for Tf = 0.062, 0.07, 0.092. The high frequency of minimization is chosen to identify nearby local

minima, separated by an energy barrier.

From the MD simulations, we obtain a time series of inherent structures. We are interested in transitions between two different inherent structures, identified by comparing two consecutive minima. We recorded 70970, 130859, and 1593359 transitions between inherent structures, for Tf = 0.062, 0.07, 0.092respectively. We wish to characterize the

potential energy barriers corresponding to the transitions. This analysis is computationally costly. Given the large number of transitions detected, we chose to analyze transitions detected at least 4 times, regardless of the direction

FIG. S1. Probability distribution of the potential energy barriers Vbsampled at temperatures TMD= 0.01and 0.04.

of the transition (A → B or B → A). The number of transitions analyzed is equal to 14195, 23535, and 117361, for Tf= 0.062, 0.07, 0.092respectively.

In order to investigate the influence of the temperature TMD on the characteristics of the double well potentials

identified, we present in Fig. S1 the probability distribution function of potential energy barriers identified with TMD= 0.01, and 0.04 (used in the main text). The sampling temperature TMDinfluences the tail of the distribution

only, which decays as exp(−Vb/TMD). We conclude that the sampling of relevant TLS is not affected by a variation

of TMDwithin a reasonable interval.

III. TUNNEL SPLITTING

For each analyzed transition, the Nudged Elastic Band (NEB) algorithm outputs a one-dimensional potential defined for the reduced coordinate ξ, between the two minima only. We run the algorithm using 40 images of the system. We need to extrapolate the potential in order to obtain a full double well potential. We tested various extrapolation schemes, such as parabolic fitting of the minima, and mirroring around each minima, defining V (−ξ) = V (ξ) for ξ < ξa and V (2 − ξ) = V (ξ) for ξ > ξa, where ξa is the coordinate of the potential maximum: V (ξa) = V (0) + Va.

In the main text, we used a linear extrapolation of the reaction path obtained with the NEB. Let us denote r1 and

r2 the coordinates of the particles in the first two images of the system along the reaction path (r1 is an energy

minimum). We measure the potential energy of the configuration, starting from r1, and moving in the direction

r1− r2. We perform a similar extrapolation at the other minimum. We show in Fig. 1 (main text) a double-well

potential obtained from the NEB algorithm (blue part), and by linear extrapolation of the reaction path (black part). We have compared all methods and found that while each scheme gives a slightly different potential, the statistics of tunnel splittings remains unaffected by our choice. In the main text, we use the most physical scheme, namely the linear extrapolation of the reaction path.

Once the classical potential V (ξ) is obtained by extrapolation as discussed above, we solve numerically the Schrödinger Eq. (2) (main text) using a standard Python package. Note that, in general, the Laplacian term should take into account curvature effects along the reaction coordinate, ∇2

ξ = ∂ξ2 + (detg)−1/2∂ξ[(detg)1/2∂i] +

(detg)−1/2_{∂}

i[(detg)1/2∂ξ], where g is a metric tensor and ξiare coordinates orthogonal to ξ. For simplicity, we neglect

these effects and use the standard second derivative along the reaction coordinate.

We present in Fig.S2a scatter plot of the tunnel splitting E as a function of participation ratio P R and energy barrier Vb for DWPs identified in glasses from hyper-quenched (top) to ultrastable (bottom). In Fig. S2 (a,c,e) we

observe that in the relevant range of E. 10−3 _{the value of P R can be as large as ∼ 200 for T}

f = 0.092 and ∼ 30

for Tf = 0.062. In Fig. S2(b,d,f) we observe that in the same relevant range, the barrier is always Vb & 10−2 E,

indicating that the relevant DWP are indeed TLS. We also checked (not shown) that in the same range, one always has E3− E1 E, where E3 is the third energy level.

Finally, we checked that for most TLS in the relevant range, the wavefunctions of the first two levels are sufficiently delocalized over the two wells, indicating that tunnelling is active. However, the barrier Vb has a relatively wide

3

FIG. S2. Scatter plot of the participation ratio P R (a,c,e) and the potential energy barrier Vb(b,d,f) versus the tunnel splitting E, of double-well potentials in glasses prepared at Tf = 0.092(a-b), Tf = 0.07(c-d), and Tf = 0.062(e-f). The data for DWPs found in the same glass sample (there are Ng of them) are presented with the same color. The tunnel splittings are computed using an adimensional mass em = 30000.

distribution (see Fig.S2), and there exist TLS with large barriers and hence very small tunnelling matrix elements. For those TLS, the wavefunctions are almost localized, indicating that tunnelling is highly suppressed. These TLS would be frozen in experimental conditions. The wide distribution of Vbis known to be responsible for a logarithmic

growth of n0with observation time τ, n0∝ log τ [S4], which might also provide an explanation for why our simulations

overestimate n0with respect to experiments (see main text).

IV. DIMENSIONAL SCALING ANALYSIS FOR UNIT CONVERSION

The number of TLS per particle in a given glass sample with a tunnel splitting less than E, for E → 0, is n0E.

Hence, n0 has the dimensions of an inverse energy, expressed in units of −1. However, because in our simulation

units the number density is ρ = 1, n0 is also the number of TLS per unit volume, in units of −1σ−3, i.e.

nexp_{0} = nsim

0 × −1σ−3 . (S1)

For Argon, −1_{σ}−3_{∼ 3.85 × 10}48_{J}−1_{m}−3_{, while for Nickel }−1_{σ}−3 _{∼ 1.51 × 10}48_{J}−1_{m}−3_{, which allows one to convert}

our numerical results for nsim

FIG. S3. The TLS density n0, as extrapolated from n(E)/E in the limit E → 0, divided by em, as a function of glass stability, encoded by the value of log(τα/τo)for the three values of Tf and different em. A reduction of n0 by two orders of magnitude is robustly observed, independently of em. Furthermore, we find n0∝ emindependently of Tf.

Because the glass transition temperature in the simulation is Tg = 0.067, the corresponding glass transition

tem-perature in physical units is

Tg = 0.067×

kB

. (S2)

Finally, the temperature TQat which quantum effects become relevant is that at which the thermal wavelength equals

the interparticle distance. Since our simulation density is ρ = 1/σ3_{, we get}

TQ=
2π~2
mσ2_{k}
B
=2π
e
m
kB
, (S3)

and we recall that em = mσ2_{/}_{~}2 _{is the dimensionless mass that appears in the Schrödinger equation. Finally, note}

that the relevant (active) TLS are those with E < kBTQ, and their total number in our simulation is given by

nactive= N Ngn (E = kBTQ) ∼ NNgnsim0 kBTQ = 2πN Ng nsim 0 e m . (S4) We find that n0/me is roughly constant for a given glass stability Tf, as shown in Fig.S3. This results implies that

the choice of emcan be quite arbitrary, within a reasonable range. In particular, emcannot be too small otherwise the condition TQ Tg would be violated.

V. VIBRATIONAL AND TLS CONTRIBUTIONS TO THE SPECIFIC HEAT

Here, we compare the contributions to specific heat coming from TLS and from harmonic vibrations around an inherent structure. To obtain the TLS contribution, for a given Tf and em, we collect all the TLS found in all the Ng

glasses, with splitting Ei, and compute [S4,S5]

CTLS= 1 N Ng X i x2 i cosh(xi)2 , xi= Ei 2kBT . (S5)

To obtain the vibrational contribution, we considered a single glass prepared at Tf = 0.062, and all the NISinherent

structures found within that glass. For each inherent structure, we diagonalize the Hessian matrix of the classical potential, to obtain a set of eigenvalues (spring constants) κα. Each of these provides a quantum harmonic oscillator

contribution to the vibrational specific heat, which is Cvib= 1 N NIS X α x2α sinh(xα)2 , xα= ~ωα 2kBT , ωα= r κα m . (S6)

5

FIG. S4. (a) TLS contribution to the specific heat per particle, as a function of T . Dotted-dashed lines are the asymptotic low-temperature scaling, CTLS ∼ T , for em = 30000 (for em = 5000the statistics is not sufficient for a good extrapolation). (b) Vibrational contribution to the specific heat per particle, as a function of T , for Tf = 0.062, averaged over inherent structures in a typical glass metabasin.

Note that the finite size of the system imposes a cutoff on the low-frequency Debye behavior. In fact, the lowest frequency found in our system is ~ωα/kB = 0.0038 (in simulation units) for em = 5000, and ~ωα/kB = 0.0016 for

e

m = 30000. To avoid this problem we used data of larger system with N = 192000 particles [S6] and extrapolate the quadratic region of the density of states to the ω → 0 limit.

Yet, from Fig.S4we conclude that the vibrational contribution decays much faster than the TLS one upon lowering
temperature, and that already at T ∼ 10−4 _{we have C}

vib CTLSfor all considered values of emand Tf.

VI. TUNNELING RATES

In this section we compute the tunneling rates of the TLS identified in our simulations. This allows us to determine if the TLS with energy splitting E . kBTQ, which we considered as “active” at T . TQ, can actually tunnel over

experimental timescales.

The characteristic time to observe a transition from the higher energy level to the lower one can be estimated from the decay rate Γ, computed within the Wentzel-Kramers-Brillouin (WKB) approximation [S7]

Γ = 1
m
Z a
0
dx
p(x)
−1
exp
"
−_{~}2
Z b
a |p(x)|dx
#
, p(x) =p2m(_{E}2− V (x)), (S7)

where [0, a] and [a, b] are the width of the higher energy well and of the energy barrier, respectively, both measured at the energy level E2. This construction is sketched in Fig.S5(a). We present in Fig. S5(b-c) the scatter plots of

the tunneling rate Γ of a DWP as a function of its energy splitting E. Each panel corresponds to a different glass stability, from ultrastable (b) to hyperquenched (d).

To compare these results to experimental timescales, we consider the parameters for NiP ( em = 30000), for which
= 6.14_{× 10}−20 _{J. Together with ~ = 1.05 × 10}−34 _{m}2_{kg/s, we get a natural frequency unit /~ ∼ 10}14 _{Hz for Γ.}

Most TLS with E < 10−3_{, which could tunnel around T}

Q, have rates Γ ≥ 10−14, which corresponds to Γ ≥ 1 Hz in

physical units. This means that most TLS identified as active based on their energy splitting would actually tunnel over experimental timescales.

VII. DISTRIBUTION OF TUNNELING MATRIX ELEMENT ∆0

In the standard TLS model, the Hamiltonian of a single tunneling state takes the form H = 1 2 ∆ ∆0 ∆0 −∆ (S8) in the localized representation. The diagonal splitting of the TLS can be estimated by

∆ = ∆V +_{~}ω2− ω1

FIG. S5. (a) Definition of the parameters a and b used in the WKB calculation of tunneling rates, Eq. (S7). (b-d) Transition rates Γ as a function of energy splitting E for different glass stabilities, Tf = 0.062(b), 0.07 (c), 0.092 (d). The data for DWPs found in the same glass sample (there are Ng of them) are presented with the same color. The rates are computed with NiP parameters ( em = 30000).

where ω1,2 are the classical frequencies in the two energy minima [S5]. The tunneling matrix element is ∆0 =

2hψL|H|ψRi, where |ψR,Li are the wave functions of the left and right wells. While this definition has been widely

used in the theoretical literature, it is not obvious how to define the localized basis |ψR,Li, and therefore not practical

to obtain a numerical evaluation of ∆0. We used instead the WKB approximation to estimate the tunneling matrix

element [S4]
∆0≈ E exp
"
−1_{~}
Z b
a |p(x)|dx
#
, _{E =} E1+E2
2 , (S10)

where here a, b, and p(x) are derived from E instead of E2 as in the calculation of Γ. Note that the most important

contribution, in both cases, comes from the exponential term. We show in Fig.S6(a) the resulting cumulative density of diagonal elements ∆ (in the same format as Fig. 3 in the main text), and probability distribution function P (∆0)

of tunneling elements, computed for each Tf. Our numerical results are consistent with the TLS model prediction

P (∆0) ∼ 1/∆0. The density of diagonal elements is constant at small ∆, also in agreement with the TLS model.

However, the condition ∆0 ∆ is not always satisfied in our data, and as a result the true splitting E is generally

larger than ∆, which results in a decrease of the plateau values of n(E)/E compared to n(∆)/∆.

SUPPLEMENTARY REFERENCES

[S1] Andrea Ninarello, Ludovic Berthier, and Daniele Coslovich, “Models and algorithms for the next generation of glass transition studies,” Physical Review X7, 021039 (2017).

[S2] Ludovic Berthier, Elijah Flenner, Christopher J Fullerton, Camille Scalliet, and Murari Singh, “Efficient swap algorithms for molecular dynamics simulations of equilibrium supercooled liquids,” Journal of Statistical Mechanics: Theory and Experiment2019, 064004 (2019).

7

(a) (b)

FIG. S6. (a) Cumulative distribution of the diagonal splitting ∆, divided by ∆ for different glass stabilites. The data is shown in a way similar to Fig. 3 of the main article. (b) Probability distribution of the off-diagonal element ∆0 for different glass stabilities. Our results are consistent with the TLS model prediction P (∆0) ∼ 1/∆0. Data obtained for em = 30000 (NiP parameters).

[S3] Arthur Q Tool, “Relation between inelastic deformability and thermal expansion of glass in its annealing range,” Journal of the American Ceramic society29, 240–253 (1946).

[S4] W A Phillips, “Two-level states in glasses,” Reports on Progress in Physics50, 1657–1708 (1987).

[S5] P. W. Anderson, B. I. Halperin, and C. M. Varma, “Anomalous low-temperature thermal properties of glasses and spin glasses,”Philosophical Magazine25, 1–9 (1972).

[S6] Lijin Wang, Andrea Ninarello, Pengfei Guan, Ludovic Berthier, Grzegorz Szamel, and Elijah Flenner, “Low-frequency vibrational modes of stable glasses,” Nature communications10, 26 (2019).

[S7] Anders Andreassen, David Farhi, William Frost, and Matthew D Schwartz, “Precision decay rate calculations in quantum field theory,” Phys. Rev. D95, 085011 (2017).